SUPERSEDED (click for Active standard)
| ||Format||Pages||Price|| |
|3||$48.00||  ADD TO CART|
1.1 This practice covers the preparation and use of Mattsson's solution of pH 7.2 as an accelerated stress-corrosion cracking test environment for brasses (copper-zinc base alloys). The variables (to the extent that these are known at present) that require control are described together with pos- sible means for controlling and standardizing these variables.
1.2 This practice is recommended only for brasses (copper-zinc base alloys). The use of this test environment is not recommended for other copper alloys since the results may be erroneous, providing completely misleading rankings. This is particularly true of alloys containing aluminum or nickel as deliberate alloying additions.
1.3 This practice is intended primarily where the test objective is to determine the relative stress-corrosion cracking susceptibility of different brasses under the same or different stress conditions or to determine the absolute degree of stress corrosion cracking susceptibility, if any, of a particular brass or brass component under one or more specific stress conditions. Other legitimate test objectives for which this test solution may be used do, of course, exist. The tensile stresses present may be known or unknown, applied or residual. The method may be applied to wrought brass products or components, brass castings, brass weldments, etc., and to all brasses. Strict environmental test conditions are stipulated for maximum assurance that apparent variations in stress-corrosion susceptibility are attributable to real variations in the material being tested or in the tensile stress level and not to environmental variations.
1.4 This practice relates solely to the preparation and control of the test environment. No attempt is made to recommend surface preparation or finish, or both, as this may vary with the test objectives. Similarly, no attempt is made to recommend particular stress-corrosion test specimen configurations or methods of applying the stress. Test specimen configurations that may be used are referenced in Practice G30 and STP425.
1.5 This standard does not purport to address all of the safety concerns, if any, associated with its use. It is the responsibility of the user of this standard to establish appropriate safety and health practices and determine the applicability of regulatory limitations prior to use. (For more specific safety hazard statements see Section 8.)
2. Referenced Documents (purchase separately) The documents listed below are referenced within the subject standard but are not provided as part of the standard.
D1193 Specification for Reagent Water
G30 Practice for Making and Using U-Bend Stress-Corrosion Test Specimens
ICS Number Code 77.060 (Corrosion of metals); 77.120.30 (Copper and copper alloys)
|Link to Active (This link will always route to the current Active version of the standard.)|
ASTM G37-98, Standard Practice for Use of Mattsson's Solution of pH 7.2 to Evaluate the Stress- Corrosion Cracking Susceptibility of Copper-Zinc Alloys, ASTM International, West Conshohocken, PA, 1998, www.astm.orgBack to Top